Applied Science and Convergence Technology 2020; 29(1): 19-22
Published online January 31, 2020
Copyright © The Korean Vacuum Society.
Jaewon Oh, Won Yeob Jeong, Seo Yun Lee, Bom Lee, and Mee-Yi Ryu*
Department of Physics, Kangwon National University, Gangwon-do 24341, Republic of Korea
This is an Open Access article distributed under the terms of the Creative Commons Attribution Non-CommercialLicense (http://creativecommons.org/licenses/by-nc/3.0) which permits unrestricted non-commercial use, distribution,and reproduction in any medium, provided the original work is properly cited.
Optical properties of methylammonium lead bromide (MAPbBr3) perovskite single crystals grown using a seed-induced inverse temperature crystallization method were studied using photoluminescence (PL) and time-resolved PL measurements. Crystallization rate was observed to be faster with an increasing crystallization temperature. The highest crystal quality was recorded for a sample crystallized at 85 °C, and it exhibited the strongest X-ray diffraction peaks and PL intensity. The PL spectra for all samples crystallized at room temperature showed an asymmetric shape with a shoulder in the low energy side; this can be attributed to a photon recycling effect caused by re-emission inside the single crystal. We confirmed that the structural and optical properties of MAPbBr3 single crystals can be manipulated by modifying the crystallization temperature.
Keywords: Perovskite, Photoluminescence, Single crystal, Time-resolved photoluminescence
In recent years, methylammonium lead halide perovskites have emerged as viable semiconductor materials in applications such as solar cells, light-emitting diodes, laser, and photodetectors [1–4]. In particular, organometal halide MAPbX3 (MA = CH3NH3, X = Cl, Br, or I) single crystals exhibit excellent optoelectronic properties including high carrier mobility, high absorption coefficient, and tunable emitting wavelength [2,5,6]. To realize large-scale, high-quality, and rapid growth rate perovskite single crystals, several methods including anti-solvent vapor-assisted crystallization, seed-induced method, and inverse temperature crystallization (ITC) have been studied [5-7].
Most of these studies focused on device characteristics and efficiency of perovskite single crystals, and little attention is given to the fundamental properties of single crystals [5–7]. To develop high-quality single crystals, asymmetrical photoluminescence (PL) emission spectra occurring in MAPbBr3 single crystals must be addressed. Yang
In this study, MAPbBr3 perovskite single crystals were synthesized using seed-induced and ITC methods at various crystallization temperatures to achieve rapid growth rates and high crystallinity. Subsequently, optical properties were evaluated using PL and timeresolved PL (TRPL) spectroscopy. With increasing crystallization temperatures, the rate of microcrystal formation increased. Thus, high-quality single crystals were synthesized with a high growth rate at 85 °C. The PL spectra showed asymmetrical shapes at room temperature, which may be attributed to the photon recycling effect that occurs inside the single crystal.
For the synthesis of MAPbBr3 perovskite single crystal samples, a 1 M solution of MA and PbBr2 was prepared in
X-ray diffraction (XRD) measurements were conducted using X’pert Pro X-ray diffractometer (Malvern Panalytical). Temperature-dependent PL measurement was performed using a spectrometer (DM500i, Dongwoo Optron Co., Ltd.) with a He-Cd laser (λ = 325 nm, Kimmon) as the excitation source. The PL spectra were recorded using a charge-coupled device detector (ANDOR DV420-BU2). The samples were mounted on a closed-cycle cryostat (CCS-150, Janis Research Co., Inc.) with the temperature ranging from 10 to 300 K. The TRPL was measured using a FLS 920 spectrometer (Edinburgh Instruments Ltd.), and a picosecond pulsed diode laser (λ = 375 nm, pulse width = 48.4 ps, EPL-375, Edinburgh Instruments Ltd.). The TRPL spectra were recorded using a time-correlated single-photon counting system.
Figure 1(a) shows images of the grown MAPbBr3 single crystal at different crystallization temperatures. The size of the crystals obtained when using the added seed-induced method was larger compared with that obtained using the general ITC method [11,12]. The largest crystal size obtained was ~63 × 59 × 25 mm3 at 85 °C. However, at crystallization temperatures greater than 90 °C, the spontaneous formation of smaller multiple crystals was observed; moreover, the crystals appeared stacked. This may be attributed to the decreasing solubility of MAPbBr3 in DMF with increasing temperature . At higher crystallization temperatures, the precursor solution becomes supersaturated, thereby producing a large number of small crystals. This prevents the seed-induced crystal from growing further. To confirm crystallinity, we performed XRD measurements at room temperature. Figure 1(b) shows the XRD spectra obtained with diffraction angles (10° to 80°). The narrow and strong diffraction peaks at 15.3°, 30.5°, 46.3°, and 63.0° correspond to the (100), (200), (300), and (400) planes of the cubic phase, respectively . As shown in Fig. 1(b), the sample crystallized at 85 °C exhibits stronger (~10 times) diffraction peaks compared to those of other samples. The full width at half maximum (FWHM) of the diffraction peaks is shown in the inset of Fig. 1(b). Except for the (100) plane, the FWHM of the diffraction peaks is the lowest in the 85 °C sample. The strong intensities and narrow linewidths are indicative of high crystallinity. Thus, we experimentally confirm that high-quality MAPbBr3 single crystals with a high growth rate can be grown using the seed-induced ITC method at 85 °C.
(Color online) (a) MAPbBr3 single crystal images at different crystallization temperatures. (b) X-ray diffraction patterns at room temperature. The inset shows the full width at half maximum (FWHM) of (100), (200), (300), and (400) planes.
Figure 2(a) illustrates the room temperature PL spectra of the MAPbBr3 single crystal samples. The PL peak positions of all samples are located at around 534 nm; for the sample obtained at 85 °C, the peak intensity is approximately three times stronger compared to that of the sample obtained at 90 °C. Thus, the PL results are in good agreement with the XRD data. However, we observed variations in the PL spectrum with changing irradiation positions of the excitation laser beam. Two spots (center of sample: spot A and edge of sample: spot B) with differences in PL peak positions are illustrated in the inset of Fig. 2(b). In the PL peak position, spot A is located at a shorter wavelength range than spot B, and the difference between the two PL peak positions is about 5 nm. To identify the change caused by the difference in the laser irradiation position, an excitation power-dependent PL experiment was performed at the two spots. The variations in the PL characteristics (peak position and relative intensity) corresponding to the power of the excitation source at the two spots showed a similar tendency (not shown here).
(Color online) (a) Room-temperature PL spectra of MAPbBr3 single crystal samples. (b) PL spectra of the sample obtained at 85 °C in different irradiation regions. The inset shows the laser irradiated region of the sample.
The PL spectra for all samples exhibit asymmetric shapes, with the shoulder located in the long-wavelength (low energy) side at room temperature. The temperature-dependent PL measurements were performed to investigate the low-energy state of PL emission. Figure 3(a) shows the temperature-dependent PL spectra measured at spot A of the 85 °C sample for the selected temperatures. MAPbBr3 single crystals are well known for phase transitions to cubic (T > 230 K), tetragonal (145 K < T < 230 K), and orthorhombic (T > 145 K) phases as the temperature decreases. Our XRD measurement was performed only at room temperature, and thus, we could not directly confirm the phase transition with the change in temperature; however, the temperature dependence of the PL peak in Fig. 3(b) shows a similar tendency to the reported results [9,10].
(Color online) Temperature-dependent (a) PL spectra, (b) PL peak positions, and (c) FWHM of the 85 °C sample on laser irradiation spot A.
The obtained PL spectra can be separated into three Gaussian peaks (T ≤ 70K) and two Gaussian peaks (T > 80 K). The PL peak energies and FWHM extracted from Gaussian fitting results are shown in Figs. 3(b) and 3(c), respectively. Similarly, a change in FWHM with increasing temperature was observed at the two peaks. This is consistent with the excitation power-dependent PL results, which suggest that the two PL emission origins are the same. The sub-peaks appearing in low-temperature regions can be attributed to the phase transition from the orthorhombic phase. At high temperatures, the main peak (Peak1) originates from band-to-band transition . However, the origin of the low-energy peak (Peak2) observed in the PL spectra at high temperatures is unclear [8,10,13].
To investigate the carrier dynamics of the shoulder peak (Peak2), TRPL measurement was conducted as a function of wavelength at room temperature. Figure 4(a) presents the PL decay curves of spot A (85 °C sample). With an increase in the emission wavelength from 515 to 563 nm, the PL decays become slower. The PL decay times of the 85 °C sample were calculated using the bi-exponential decay function
(Color online) (a) PL decay curves of spot A and PL decay times of (b) spot A and (c) spot B as a function of emission wavelength. The measured PL spectrum and fitted PL peaks are also shown.
We investigated the influence of crystallization temperatures on the optical properties of MAPbBr3 perovskite single crystals using PL and TRPL measurements. It was found that an increase in the crystallization temperatures (from 80–100 °C) led to the formation of multiple microcrystals. We confirmed that the optimal crystallization temperature was 85 °C in the seed-induced ITC method. All samples exhibited asymmetric PL spectra at room temperature; moreover, the two separated PL emissions showed similar characteristics as a function of excitation laser power and temperature. The PL peak on the low energy side at high temperatures was explained by the re-emission originating at the edge of the crystal due to the self-absorption and reflection inside the bulk.
This research was supported by the Basic Science Research Program through the National Research Foundation of Korea (NRF) funded by the Ministry of Education, Science, and Technology (NRF-2019R1A2C1086813) and Supporting Business for College Innovation from Kangwon National University. Time-resolved photoluminescence measurements were performed at the Central Lab of Kangwon National University.